advertisement

MAGNETIC PERMEABILITY AND EDDY-CURRENT MEASUREMENTS James H. Rose, Erol Uzal and John C. Moulder Center for Nondestructive Evaluation Iowa State University Ames, IA 500ll INTRODUCTION The calculation of the impedance of a right-cylindrical air-core coil placed next to a flat plate of a uniform polycrystalline metal alloy is a canonical problem in quantitative eddy-current inspection. Cheng [1] and Dodd and Deeds [2] proposed a widely-used solution for a coil next to a semi-infinite half-space of metal, which agrees quantitatively with impedance measurements made for a wide variety of thick but nonmagnetic metal plates. Said plates were assumed to have a uniform and frequency-independent conductivity, cr. The same authors proposed a similar solution for ferromagnetic metals (such as iron, steel and nickel), characterized by both a uniform cr and a nontrivial uniform permeability /l. In this paper, we report quantitative measurements of the impedance of rightcylindrical air-core coils placed next to well-characterized thick plates of commercially pure Ni and Fe as well as Ni-Fe alloys and a variety of medium carbon (nominally type 1090) steels used as rails. We compare the results of our measurements with calculations [1,2] for coils next to half-spaces that have an otherwise uniform, frequency-independent !l and cr. Large discrepancies between the measurements and calculations are reported. Ferromagnetic polycrystalline metals are generally idealized as structureless continua for the purpose of analyzing eddy-current data. Material properties enter via a frequency independent conductivity cr and the nonlinear relation between the magnetic induction and the magnetic field, B=B(H). Magnetic fields used for eddy-current inspection are generally weak and it is generally assumed that B and H are linearly related via the initial permeability J B(r, w) = d 3r' ~(r,r' ,w)· H(r' ,w) Here, I::!:. (1) is a tensor (possibly complex) that is in general a function of the position coordinates, r and r', and the angular frequency roo Many authors further assume that Review of Progress in QuantitaJive Nondestructive Evaluation. Vol. 14 Edited by D.O. Thompson and D.E. Chimenti. Plenum Press. New York, 1995 I::!:. 315 is isotropic, i.e. proportional to the unit tensor. If one now further assumes that #:. is a local, constant and frequency-independent function, i. e. l;!,(r,r', OJ) = Ill, (2) we obtain the model mentioned in the first paragraph. There are obviously many places where errors can intrude to belie the idealization described above. The existence of discrepancies between theory and experiment is not unexpected, given the simplifYing assumptions made by idealizing the magnetic properties of the plate in terms ofa permeability that is independent of both frequency and position. We will discuss the possibility of improving the agreement between theory and experiment by removing one or the other of these simplifications. The structure of this article is as follows. First, we introduce the calculation method. Second, we describe the measurement system. Third, we present the results and our data analysis. Fourth, we assume that !l is constant throughout the sample, but may depend on the frequency, and extract a frequency-dependent !l for f= I kHz to 200 kHz. These estimated values of the frequency-dependent permeability are significantly less than either measured or handbook values of the dc permeability. Finally we conclude the paper with a brief summary and discussion. THEORETICAL MODEL The measurements that will be reported below were modeled as follows. We imagine a semi-infinite half-space of metal that is characterized by an otherwise uniform, real, frequency-independent conductivity and permeability, a and!l. A right-cylindrical coil is imagined next to the planar interface that separates the metal and free space. The conductivity offree space is taken to be zero, while the permeability offree-space is denoted by !lo. We further imagine that the impedance of the coil is obtained for this configuration, as well as for the coil in free-space alone. The difference of these two measurements (i.e., the change in impedance caused by placing the probe next to the metal) is modeled by (3) Here, !lR = !l / !lo is defined to be the relative permeability, while u 1 (the wave vector in the metal) is given by (4) The dimensions of the coil enter in the functions M, A and K, which are defined next. First, f x.Mx)dx fir, M( a) == (5) 316 where r I and r2 denote the inner and outer radii of the coil. Second A(a) == (e- dli - e- dl , ) , (6) where hi denotes the height of the bottom of the coil above the metal (i.e., the lift oft) and ~ denotes the height of the top of the coil. Finally, (7) where n denotes the number ofturns of wire that constitute the coil, and L = ~ - hi. IMPEDANCE MEASUREMENTS Measurements were performed using an automated eddy-current work station [3]. The complex impedance of the coil was determined with a Hewlett Packard HP 4194A impedance analyzer. Measurements were made at 100 equally-spaced frequencies that ranged from 1 to 300 kHz. Two precision-wound and nearly right-cylindrical coils were used as probes. The first, denoted Probe A, was relatively large; the second was smaller and denoted Probe L. Measurements were taken first with the probe in air, then with the probe in firm contact with the surface of the specimen. Data are reported here as the difference of the two complex impedances, I'!.Z=Z metal - Zai<. Since we are interested in the initial permeability of the samples, it is important that the magnetic fields produced by the coils should be sufficiently weak that the relation between Band H is linear. In fact, the computed values of the coil's magnetic field are quite small «1 Oe). Furthermore, we measured the impedance of the nickel sample using input currents that varied in magnitude by a factor often. The resulting impedances were found to be independent of the amplitude of the current, which confirms the required linearity. The dimensions of the coils are given in Table 1. SPECIMENS Samples consisted, in part, of several 99.99% commercially pure nickel rods that were all cut from the same bar of material. One rod was then fashioned into a ring suitable for use as a transformer. After cutting, the Ni samples were vacuum annealed for two hours at a temperature of 1073 kelvins and furnace cooled. The Ni samples were also carefully demagnetized. A very low frequency ( 0.03 Hz), transformer-based measurement was used to determine the relative initial permeability of the Ni ring sample. The result was found to be PR ~ 300. Other samples were obtained from metal specimens that were readily available and include 99.99% commercially pure iron, a variety oflow carbon steels, as well as two iron-nickel alloys, Fe(3% Ni) and Fe(46%Ni). These other samples were measured in the "as is" condition, i.e., no attempt was made to anneal or demagnetize them. Table 2 lists the samples, their conductivity and "handbook" values of the relative initial permeability. The last column lists values of the relative initial permeability as estimated from the impedance measurements; these data will be discussed more extensively below. 317 Table 1. Geometry of the coils used. L 235 1.07mm 2.62mm 0.62mm 2.93mm A 504 7.6mm 11.27 mm 0.125 mm 2.42mm Probe Number ofTums, n Inner Diameter, 2 r l Outer Diameter, 2 r 2 Lift OH: hI Coil Length, L Table 2. List of samples, their resistivities, handbook ~R and estimated ~R . Sample Ni(99.99%) Fe (ARMCO) Fe(3%Ni) Fe(46%Ni) Nominal Resistivity (10- 8 n.m) Handbook Relative Initial Permeability ~R ~R 8.9 7.2 12 40 400 250 135 90 3000-6000 100-125 - Estimated Relative Initial Permeability - RESULTS Measured values of the imaginary component of the impedance are plotted as a function of frequency in Fig. 1 for Ni, Fe(3%Ni), Fe(46%Ni) and for AI, which is a nonmagnetic metal. The reactance of the ferromagnetic samples is positive and increases at relatively low frequencies; at higher frequencies the reactance begins to decrease, crosses zero, and then becomes increasingly negative. In contrast, the reactance of the nonmagnetic aluminum sample is never positive and becomes increasingly negative as the frequency increases. The positive-going portion of the curve and the zero-crossing are signatures of the ferromagnetic nature of the sample and will be used to estimate the relative initial permeability. The real (resistive) component of the impedance was observed to be a simple, monotonically increasing function of the frequency that was relatively insensitive to the magnetic nature of the sample. It will not be displayed or discussed further in this brief paper for lack of space. We also studied the theoretical model (Eqs. 1 - 7) of the coil's impedance, which assumed a frequency-independent and spatially-constant relative permeability. We found that the general features of the impedance described in the last paragraph were reproduced by the model. In addition, we found that for the frequencies and coils used in this study, the impedance is predicted to depend, very nearly, solely upon the ratio WO", a fact that was noted earlier by Dobmann et al. [4]. Furthermore, we found that the frequency of the zero-crossing depends almost linearly upon WO". Hence, the model suggests a method for determining WO", once the zero-crossing frequency is known. Figure 2 shows that the measured impedance is inconsistent with our model calculation. This figure compares the measured value of the impedance of coil A for the Ni sample with the results computed from the model using the measured static value of the relative permeability, IlR = 300. The curves are markedly different; e.g., the experimental 318 --- 1000 -.---e--.- Nickel 3%Ni Fe 46°.4Ni Fe 7075 AI o o 100000 200000 Frequency, Hz 300000 Figure l. Shows the imaginary part of the impedance of Probe A for samples listed in Table 2, for frequencies ranging from 10 kHz to 300 kHz. curve reaches a relative maximum of + 100 n and crosses zero at 135 kHz, while the theoretical curve reaches a relative maximum of 220 n and crosses zero at> 300 kHz. On the other hand, both curves share the same general shape. These results seem clearly to invalidate a model that assumes the permeability is spatially uniform inside the plate and independent of frequency from 0.03 Hz to 300 kHz. ! 200 O~----------------~----------------~~~ ~ S' -200 ..... 'il ~ ] -400 -6ooL-----5~0~~~1~0-0~--~15~0--~~20~0----~2~50~--~300 Frequency (kHz) Figure 2. Shows the measured and calculated changes in the reactance of a coil placed next to the flat end of a vacuum annealed and carefully demagnetized Ni rod. The static relative initial permeability of 300 was measured independently. 319 200 ~ } .. O~------------~~~----------------~ -200 ~ -400 J -600 50 100 150 200 250 300 Frequency (kHz) Figure 3. Shows the measured and calculated changes in the reactance of a coil placed next to the flat end of a vacuum annealed and carefully demagnetized Ni rod. The relative permeability of 145 used in the theory was fit to the experimental data. We also determined the spatially uniform and frequency-independent permeability that best fit the zero-crossing in the Ni data. Figure 3 shows the fit to the experimental data when the relative permeability is assumed to take the value of 145. As is evident, even though the calculated values of the impedances are somewhat smaller than the experiment, the fit is reasonably good. Table 2 lists the relative permeability estimated in this way for the Ni, Fe and FelNi alloys that we studied. In each case the fitting value for the relative permeability is much less than the handbook value. In the case of Fe( 46%Ni), the handbook value of the permeability is between 3000 and 6000, while our fitting value was much smaller, 100 - 125. FREQUENCY-DEPENDENT PERMEABILITY? We have found, as shown in Fig. 2, that it is impossible to fit the measured impedance between 10 and 300 kHz using the permeability measured at 1/30 Hz. There are many idealizations of the magnetic properties involved in obtaining the model used for the calculations, e.g., (1) frequency independence, (2) spatial uniformity, and (3) spatial isotropy. It would be reasonable to relax each of these assumptions independently to determine whether one of them provides the dominant contribution to the discrepancy between theory and experiment. We will begin this study in the final part of this paper, where we assume that the permeability depends on the frequency, and is consequently a complex quantity. However, we continue to assume that the permeability is spatially uniform and isotropic throughout the plate. That is, (8) Our purpose is to extract the hypothesized frequency-dependent complex permeability at each frequency from the measured real and imaginary parts of the 320 impedance. We determined III and IlR by computing /t,.Z from Eq. 3 using Eq. 8, and fitting the result to the data at each frequency. The real part of the permeability, as determined above, for the demagnetized and vacuum annealed Ni sample is shown in Fig. 4. Measurements were made with two different samples, both prepared in the same way. In addition, measurements were made with both the relatively large Probe A and the relatively small Probe L. For frequencies above 10 kHz, the results were completely consistent. They show an estimate for IlR of approximately 165 at 10 kHz. This estimate decreases smoothly and monotonically to IlR =140 at 200 kHz. These estimated values of the permeability are consistent with the value of 135 that was obtained by fitting the measured data to a frequency-independent permeability as shown in Fig. 3. Some drop offin the estimated permeability occurs at the very lowest frequencies (especially for Probe L). This decrease in apparent permeability arises owing to a loss of accuracy in the data fitting method; these values must be considered unreliable and are only shown to illustrate the difficulties that arise at low frequencies. These problems can be systematically removed by using larger coils. The estimated low frequency (1130 Hz) permeability is 300 and is shown on the y-axis. The large difference between the low frequency permeability and the eddy-current estimates for Il are unexplained. If the model of a frequency-dependent but spatially uniform permeability is accurate, we surmise that the permeability may increase by a factor of two as the frequency is decreased from 10kHz. Finally, estimates of the permeability for a variety of medium carbon rail steels are shown in Fig. 5. Estimated permeabilities were relatively independent of frequency and ranged from 40 to 70. 400 1 Low Frequency Value >- :t= :0 <0 CD ! 200 ----j E L- CD BB6 @ ~ "" . . ~ 0 ~ 0 ~ ~ ~ a.. CD > ~ Q) o 0:: "" Ni Spec. #1, L Probe D Ni Spec. #1, A Probe o Ni Spec. #2, A Probe -200 o 100000 200000 Frequency, Hz 300000 Figure 4. Shows real part of the relative initial permeability for 99.99% commercial Ni that was vacuum annealed and demagnetized. 321 70 Steel Sources Used Cr-Mo -'=' :.0 ('II --B- 60 Q) \lVheeling-Pitt Cr-Mo -&- eFI Cr-Mo --+- E --.- Q) ----.- Q) a.. .~ 1U Q) 50 40 Both Std. C Algoma Cr-V ---e- NKKHH ~ VVheeling-Pitt IS -V- 0::: British 1% Cr --e- Krupp Cr-V Beth MH -+- Sacilor Strech ~ Nippon HHSC Beth FHT -+~~,----,-----,----,----,----, o 40000 80000 Frequency, Hz 120000 Figure 5. Shows the real part of the estimated relative initial permeability for a variety of medium carbon steels. SUMMARY From this study, two principal conclusions emerge: first, handbook values of the relative initial permeability are inappropriate for quantitative modeling of eddy-current inspection of ferromagnetic metals. Second, static values of the initial relative permeability are also inappropriate. These conclusions lead us to pose the following, open question: ''How does one estimate the eddy-current skin depth in ferromagnetic metals?" ACKNOWLEDGMENT This work was supported by the NSF/ill Center for NOE at Iowa State University. We thank Mr. Michael Devine and Dr. David Jiles for help in preparing the nickel sample and for measuring its low-frequency, relative initial permeability. REFERENCES 1. D. H. S. Cheng, IEEE Trans. Instrumentation and Meas. IM-14, 107 (1965) 2. C. V. Dodd and W. E. Deeds, J. Appl. Phys 39, 2829 (1968). 3. J. C. Moulder, E. Uzal, and J. H. Rose, Rev. Sci. Instrum 63, 3455 (1992). 4. G. Dobmann, R. Becker, and C. Rodner, "Quantitative eddy current variants for micromagnetic microstructure multiparameter analysis (3MA)" in Review of Progress in Quantitative NDE, Vol. 7, eds. D. O. Thompson and D. E. Chimenti (Plenum, New York, 1988), p. 1703. 322